# Microstructural Path Analysis of Martensite martensite transformation during or after processing....

date post

28-Jun-2020Category

## Documents

view

3download

0

Embed Size (px)

### Transcript of Microstructural Path Analysis of Martensite martensite transformation during or after processing....

DOI: http://dx.doi.org/10.1590/1516-1439.000215 Materials Research. 2015; 18(3): 595-601 © 2015

*e-mail: prrios@id.uff.br

1. Introduction The microstructure of martensite is of fundamental

and practical interest because many steels of industrial importance derive their engineering properties from martensite transformation during or after processing. Historically, the martensite transformation in steels has been deemed time-independent (“athermal”). The transformation proceeds upon cooling by successive nucleation events assisted by autocatalysis1,2 that influences the intra-grain transformation, i. e. “fill-in”, as well as promotes inter- grain transformation, i. e. “spread”1,2. The propagation of martensite comprising nucleation and growth is nucleation controlled. The growth is usually very fast. Growth stops when the unit reaches a certain size delimited by impingement and/or by the austenite plasticity3,4. Coarsening is not observed. Martensite is a displacive transformation so that the product-units cannot cross high-angle boundaries, thus they remain confined to the grains where they propagate. Nonetheless, the midribs of two impinging units may cross if the stress field on impingement suffices to induce nucleation of the same martensite variant across the impinged unit as observed by Okamoto and co-workers5 in a Fe- 31wt%Ni-0.28wt%C alloy.

The elastic strain energy of a martensite unit, proportional to its aspect ratio, has major influence on the microstructure development. This energy is very high, and relaxation occurs by plastic deformation within the martensite, the invariant-shear, in the surrounding austenite as well as by the transformation of self-accommodating groups of martensite-units6. As consequence of the latter, the aspect ratio of the units observed in a microstructure tends to be coarser than expected from propagation intrinsic mechanisms.

These intrinsic aspects of martensite growth have been considered from different points of view7-15. However, the linkage to a formal description of the progress of martensite transformation as a function of the leading variable still deserves effort, minding the microstructural complexity of martensite, an example of which is shown in Figure 1.

Likewise other phase transformations, the progress of the martensite is generally expressed by the volume fraction transformed as a function of a variable related to the progress or advancement of the transformation, such as, temperature, strain or time. Nonetheless, that is not always sufficient for process-design, or for delving mechanisms, or for advanced-materials development. A better approach was proposed by DeHoff16. DeHoff introduced the concept of microstructural path to characterize the sequence of states that a system goes through during a phase transformation. His idea was subsequently developed into a fully-fledged analytical methodology, the microstructural path method, MPM, by Vandermeer and co-workers17. The microstructural path method has been employed in recrystallization as well as in diffusional transformation studies. The microstructural path function for recrystallization is represented by Ψ(SV , SV ) = KΨ where VV is the volume fraction of the product phase, SV is the area per unit volume of product-matrix interfaces, and KΨ is a parameter linked to the mechanism of the transformation. A similar approach was used by the present authors to analyze the autocatalytic “spread” of martensite from a few initially transformed grains to their untransformed neighbors18,19. In the present work, we move another step to apply the microstructural path method to consider intrinsic aspects of the martensite transformation.

Microstructural Path Analysis of Martensite Dimensions in FeNiC and FeC Alloys

José Roberto Costa Guimarãesa*, Paulo Rangel Riosa

aEscola de Engenharia Industrial Metalúrgica de Volta Redonda, Universidade Federal Fluminense - UFF, Av. dos Trabalhadores, 420, CEP 27255-125, Volta Redonda, RJ, Brasil

Received: March 31, 2015; Revised: April 17, 2015

The properties of steels that undergo martensite transformation after or during processing depend on characteristics and arrangement of martensite units within the microstructure. In this work, the global microstructure descriptors of martensite transformation are related to the individual dimensions of the martensite units, the “intrinsic dimensions”, – radius, thickness and aspect ratio – compensated for interactions among those units. In other words, the dimensions a martensite unit would have if it grew without impingement. This is accomplished by means of the microstructural path method. The methodology was applied to experimental data of martensite transformation in FeNiC and FeC alloys. The analysis of martensite dimensions permitted observing that the microstructural path of martensite includes a thermally activated step. We conclude that this thermally activated step does not mean that martensite itself has thermally activated growth step but that arrest of the martensite thickening process, owing to dislocation interaction with the interface motion may be thermally activated.

Keywords: martensitic phase transformation, microstructure, analytical methods

Guimarães & Rios596 Materials Research

2. Formal Description of Martensite Microstructural Path The microstructural path method may be expressed in real

or in “extended space”. The latter is a concept due to (JMAK) Johnson-Mehl, Avrami and Kolmogorov20-22 to analyze classical nucleation and growth of shape-preserved transformations that are randomly-nucleated. In the present work, we apply the “extended space” concept to characterize the martensite transformation in the absence of interaction with other units to relax the shape strain. Recently, the JMAK type problem has received rigorous mathematical treatment falling within the class of the so-called “birth-and-growth” processes23,24. Recently, Rios & Villa23 revisited and generalized the early JMAK theory. Rios and Villa showed that Poisson point processes and Boolean models are the essential mathematical ingredients underlying modern treatment of JMAK process. Nonetheless, in what follows, even though we bear in mind Rios and Villa results, we continue to adopt the classical terminology of the Metallurgy and Materials Science field.

The martensite product-units exhibit well defined morphologies and crystallographic habit, so that shape is preserved. The initial martensite nucleation is promoted by defects (“embryos”) pre-existent in the austenite, and proceeds autocatalytically. That is, the first unit to propagate yields a local transformation-burst that fills-in that austenite grain. The impingement of a unit on a grain boundary is capable of spreading the transformation into next grain and so forth. Such spread-event results in a cluster of partially transformed grains. Since those pre-existent embryos are scarce and randomly distributed throughout the austenite grains25, randomness also underlies the clusters resultant from the initial propagations at temperature, T. The crystallographic-variants of the martensite units observed in a grain are delimited by variant-selection to accommodate transformation strains6. Nevertheless, since neighbor grains have different orientations, aligned martensite microstructures are hardly observed in real space so that it is admissible that the randomness of those embryos that initiate different spread-events also underlies the martensite units therein - see

Figure 1. Therefore, although the martensitic transformation might not entirely fulfill the JMAK assumptions20-22, their equations will be used here as reasonable approximations. See Nok Chiu et al.24 for a more in depth mathematical discussion of usage of Boolean models in practical situations. Admittedly, the results therefrom derived here will need a careful evaluation.

Henceforth, consider the microstructure of a material containing NV disc-shaped martensite units per unit volume comprising the volume fraction transformed, VV, and the volume density of martensite-austenite interfaces, SV. These two descriptors are readily obtainable by point and lineal counting on the actual microstructure. The subscript “i” is used to mark descriptors of the dimensions of a martensite unit in extended space that can be called “intrinsic dimensions”. Proceeding, the extended volume fraction transformed, VVE, as a function of the NV units is

VVE = vi NV (1)

where vi is the intrinsic volume of a martensite unit. For disc-shaped martensite,

3 4 π

= αi i iv d (2)

where di and αi are, respectively, the intrinsic diameter and the aspect ratio of a martensite unit formed at temperature T. Substituting Equation 2 into Equation 1, using JMAK’s equation VV = 1 – exp(–VVE), and rearranging terms

1

3 ln(1 )4 −−

α = π

V i

i V

V d N

(3)

Since = ⋅αi i it d , 1

2 ln(1 )4 −−

= π ⋅

V i

i V

Vt d N

(4)

Recalling that SV = SVE(1–VV) where SVE=2πr i2NV, one obtains

3 3/2 12 2 (1 ) ln(1 )−α = = π − −i i i V V V Vt r N S V V (5)

12(1 ) ln(1 )−= − −i V V Vt V V S (6) and

2 (1 )= π −i V V Vd S N V (7)

Similarly to the microstructural path analysis conducted during recrystalization and/or diffusional phase transformations, the intrinsic dimensions correspond to the dimensions of a unit or of a single transformed region in the absence of impingement. In other words, the intr

*View more*